Photocatalytic Scheme with External Magnetic Field on Coffee Waste in Hydrogen Production

Photocatalytic is considered a deadlock-breaking technology for renewable energy and lowering environmental pollutants. Photocatalytic efficiency efforts are improved by activating the photocatalyst to introduce an external magnetic field. This review highlights recent breakthroughs by comparing original coffee waste, activation of coffee waste with the addition of catalysts, and manipulation of spin electrons by applying external magnets. Characterization was done with FTIR to look at chemical bonds, UV-Vis with Tauc's Relation approach to measure bandgap, and material morphology using SEM EDX. The increase in photocatalyst activation aligns with the decrease in bandgap value. The rate of decline in bandgap is in line with the rate of acceleration of hydrogen production. Adding an external magnetic increases hydrogen production up to 1.5 times greater than the original photocatalytic. Copyright


I. Introduction
The main focus of the world today is to develop sustainable transitional energy with priority access in terms of technology and funding [1].The construction of hydropower, wind, and wave energy plants is an application in supporting renewable energy [2], [3].However, the need for funds is significant, and it needs research and development of renewable energy that is easily applied and accessed by the community.
Photocatalytic is the process of absorbing photons from solar energy by a photocatalyst to separate H2O into H2 and O2 [4].Photons can inhibit hole and electron recombination in the photocatalyst to maximize Oxygen Evolution Reaction (OER) and Hydrogen Evolution Reaction (HER) [5].The efficiency of oxidation and reduction reactions in water can be measured through bandgap energy.The smaller bandgap distance facilitates the release of electrons in the conduction band and reduces hydrogen bonds to break covalent bonds at H2O [6].Therefore, it is necessary to present the use of solar energy to be converted into renewable energy, namely hydrogen energy.
Photocatalytic performance is limited by several factors: (1) light absorption, (2) surface redox reactions, and (3) photogeneration separation [7]- [9].Such factors are reached through doping and defects, surface structure, and charge separation efficiency via heterojunctions [10].In addition, the addition of an external magnetic field to the water separation process in hydrogen production was successfully created through the electrolysis process.The magnetic field can induce Lorentz to separate anions and cations and adjust the electronic configuration, i.e., the spin orientation of electrons [6].However, charge separation in electrolysis requires a continuous supply of electrical energy, generally accompanied by complicated devices and high energy purchase costs.Then, it requires material treatment that is easy to apply and inexpensive materials.
The main focus today is the emphasis on recycling household wastewater with hydrothermal processes in the formation of photocatalysts.Coffee waste represents one of the Persistent Organic Pollutants (POPs) in the form of a solution.POPs can be photosensitizers in absorbing UV wavelengths and photocatalysts in producing bandgap [11].The formation of photocatalysts from waste into carbon, graphite, and graphene structures continues to be carried out today.Hydrothermal is a method that is easy to apply, relatively inexpensive, and uses no complicated tools.In this study, coffee will be activated as a photocatalyst.Measurements of hydrogen production are measured in a photocatalytic process.

Material
Materials of Arabica (AR) and Robusta (RB) coffee were obtained from Aceh Gayo plantations in Indonesia.All reagents used commercial materials without further purification and were filtered using a size of 200 mesh.AR and RB were formed with the addition of 350 ml of deionized water and NaOH (75%, supplied by Sigma Aldrich) stratified variations (original, 10 mol, 20 mol, 30 mol, and 40 mol).Each reagent was then centrifuged for 1 hour and then dried at 280C for 2 hours.All reagents were washed using water and ethanol.The desorption adsorption equilibrium between the reagent and water was set in the dark for 30 minutes.

Material Characterization
Optical absorption was tested with UV-Vis reflection spectra in the range of 200 -800 nm (Specord 200 Plus Analytic Jena UV-Vis Spectrophotometer).The energy band gap (Eg) is obtained through Tauc's Relation approach, as in equation 1.
Where α is the absorption coefficient of the semiconductor represented by, hv is the energy of the photon, and A is the constant.The value of n depends on the type of optical transition of the semiconductor (n=1 for direct transition and n=4 for indirect transition) [12], [13].
Determination of functional groups was tested using IRPrestige21, Fourier Transformation Infrared/FTIR (Shimadzu, Japan).Absorbance measurements occur in the infrared radiation range to determine changes in the composition of structures and molecules that occur.Morphological samples of materials and elements using the FEI Inspect S50 testing tool with Energy Dispersive X-ray (EDX).SEM results were analyzed using ImageJ software with accumulated 3D surface plots where data processing was based on dots in each pixel.

Photocatalytic Experiments
500 W halogen lamp with calibration of light wavelength measurement was conducted using Aurora 4000 spectrometer (Changchun, China) with spectral range 350 -1100 nm and light intensity 4000-5600 counts.Visible lighting was done using a focus lens only about the photocatalyst and was controlled at a temperature of 30C for 7200 seconds.An external fixed magnet was added to the experimental apparatus installation, as shown -in Figure 1.
The MQ-8 sensor, as a hydrogen sensor, has 4 input voltages that are directly related to VCC DC 5V.There is a microtube made of Al2O3 with a crossing mechanism between the heater and Au-Pt electrodes and a gas sensing layer made of SnO2.This electrode and sensing gas are connected to VRL, which will convert and connect on an analog read.The potential difference read in analog read will cause obstacles detected in RL connected to digital read.The RL resistance consists of RS/RO, where the RS sensor resistance is at 1000 ppm H2, and the RO sensor resistance is in the test.So, the calibration of RS at 1000 ppm H2 on the sensor needs to be done to compare with the measurement results.

Results Characteristics and Morphology of Waste Coffee
FTIR tests bonding characteristics on AR and RB materials, as shown in Figure 2. The absorption at 2900 cm -1 is naturally owned by AR and RB, namely alkyl groups.The alkyl group is a CH group owned by aromatic organics clarified by the absorption of C=C-C aromatic ring stretch between 1450-1615 cm -1 .After combining with water, AR and RB show OH bonds at 3000 cm -1 -3500 cm -1 absorption.
The morphological characteristics of AR and RB were analyzed using SEM, as shown in Figure 3.The hydrothermal process in AR and RB shows the structure of natural porosity, as seen in Figure 3(a)(b).Adding NaOH catalyst increases porosity structure, as shown in Figure 3(c)(d).Maximum observation with 3D Surface Plot ImageJ processing is done to see the gradient of positive and negative peaks in the field of view, as seen in Figure 4.It can be seen that AR with hydrothermal structure has less porosity than AR with the addition of NaOH catalyst, respectively, in the image.This happened again with RB with the addition of NaOH catalysts, respectively, in the image.In each AR and RB after the addition of the catalyst, the presence of increased negative peaks indicates the presence of aromatic carbon [6], [14], [15].This is supported by the EDX results, where the amount of carbon increases after activation of the NaOH catalyst, as shown in Table 1.into hydroxyl.At the same time, the electron jump in the valence band will reduce water to produce hydron.This hydron is the forerunner of hydrogen gas.Rapid recombination of photocatalysts reduces the efficiency of oxidation-reduction reactions.One result is the small amount of hydrogen formed.The addition of external magnets is the most hotly discussed issue.External magnetism is a magnetic field where the amount of charge, speed, and strength of the magnet determines the Lorentz Force.In photocatalytics, holes and electrons are excited by photons.When holes and electrons move because they are affected by the external magnetic field, they will undergo opposite forces.As a result, the recombination of holes and electrons will be inhibited.This is evidenced by increased hydrogen AR and RB production when the photocatalytic process is coupled with external magnets.As shown in Figures 6(c) and 6(d), the increase in hydrogen production for AR and RB is almost 1.5 times compared to the original photocatalytic.

IV. Conclusions
The formation of photocatalysts from coffee waste was successfully carried out by hydrothermal method.Activation of photocatalysts using NaOH affects the bandgap value.Increased molarity tends to result in a smaller bandgap of coffee waste.This can be seen by the emergence of aromatic organics in the form of porosity, and the value of the amount of carbon increases.The bandgap reduction rate can be in line with the rate of acceleration of hydrogen production, where time is getting shorter.However, this does not affect the amount of hydrogen produced.The production of hydrogen with the addition of external magnets affects up to 1.5 times greater than the original photocatalytic.

Table 1 .
EDX Results Alphanoda et al. (Photocatalytic with External Magnetic Field on Coffee Waste in Hydrogen Production)